Presentation on theme: "Simulations of sub-100nm strained Si MOSFETs with high- gate stacks"— Presentation transcript:
1Simulations of sub-100nm strained Si MOSFETs with high- gate stacks Lianfeng Yang, Jeremy Watling*, Fikru Adamu-Lema,Asen Asenov and John BarkerDevice Modelling Group,University of GlasgowTel: Fax:10th International Workshop onComputational Electronics (IWCE-10)24th - 27th October 2004
2Outline Introduction Device structure Device Calibration (Conventional and strained Si n-MOSFETs)Device CalibrationHigh- dielectricsResults and discussionConclusions
3Introduction High- dielectrics Scaling of MOSFETs beyond the 45nm technology node expected by 2010 (ITRS), requires extremely thin SiO2 gate oxides (~0.7nm) resulting in intolerably high gate leakage.Maximise gate capacitance:The leading contenders at present are HfO2 and Al2O3. However, there is a fundamental drawback due to the resulting mobility degradation.Strained SiHas already demonstrated significant enhancement for CMOS applications.
4Gate Leakage current density due to gate tunnelling From ITRS 2003 edition
5Mobility enhancement in strained Si Our ensemble Monte Carlo simulator includes all relevant scattering mechanisms:optical intervalley phonon, inelastic acoustic phonon, ionized impurity,along with interface roughness scattering. The simulator has been thoroughly calibrated for bulk Si transport.Monte-Carlo calculation of the low-field in- and out-of-plane electron mobilities in strained Si as a function of Ge content within the SiGe buffer; inset shows the in and out-of-plane directions.
7Strained Si with high- dielectrics IBM demonstrated the high performance of strained silicon (30% enhancement) with low leakage of high- insulators (1000 lower leakage) for maximum performance with minimum standby powerIntel presented their high- on strained Si technology at IEDM 2003Source: IBM (VLSI 2002)
8Simulation of 67nm IBM Relaxed and Strained Si n-MOSFET Comparison between n-type Strained Si and control Si MOSFETs:67nm effective channel lengthSimilar processing and the same doping conditionsIn the strained Si MOSFET:10nm tensile strained Si layerStrained Si on relaxed SiGe(Ge content: 15%)K.Rim, et. al., Symposium on VLSI Technology 2001
9Strained Si n-channel MOSFET Structure Comparison between the n-type Strained Si and control Si MOSFETs:67nm effective channel lengthSimilar processing and doping conditionsOxide thickness, tox =2.2nm (SiO2)For the strained Si MOSFET:10nm strained Si layer thicknessStrained Si on relaxed SiGe(Ge content: 15%)SiGe n-MOSFET >35% drive current enhancement(70% high field mobility enhancement)
10Device Calibration – Drift Diffusion Drift-diffusion (MEDICI™) device simulationsConcentration dependent, Caughy-Thomas and perpendicular field dependent mobility modelsCorrected Si/SiGe heterostructure parameters: band gap and band offsets, effective mass, DoS and permittivity†We have used carefully calibrated Drift Diffusion simulations (MEDIC) to reverse engineered the doping profile and structure. We have carefully corrected the important bandstructure parameters, to allow for the strain etc.See:-L. Yang, J. R. Watling, R. C. W. Wilkins, M. Boriçi, J. R. Barker, A. Asenov and S. Roy, “Si/SiGe Heterostructure Parameters for Device Simulations”, accepted for publication Semiconductor Science and Technology (2004)Calibrated ID-VG characteristics of the 67nm n-type bulk Si and strained Si MOSFETs (experimental data from Rim VLSI’01)† L. Yang, et al, ‘Si/SiGe Heterostructure Parameters for Device Simulations’,to Semiconductor Science and Technology 19, p (2004)
11Device Calibration – Monte Carlo Calibrated ID-VG characteristics for 67nm conventional Si and strained MOSFETs, comparison with experimental data of Rim.Smoother interface for strained Si/SiO2 interface.See L. Yang et al, Proceedings of the 5th European Workshop on Ultimate Integration of Silicon (ULIS04), p23-26, IMEC 2004
13High- dielectrics Leakage “Ideal” high- films: thermally stable, free from electron and interface traps, leakage-free, reliable and reproducible, etc.ScalabilityLeakageReplace SiO2Quantity/DielectricSiO2Al2O3HfO2o3.9012.5322.00∞2.503.205.03TO1 (meV)55.6048.1812.40TO2 (meV)138.1071.4148.35SO1 (meV)57.1053.1016.70SO2 (meV)140.7082.3350.60Fischetti, JAP’01Ionic polarizationElectronic polarization /EgHighly polarized “soft” metal-oxygen bondswhich screen external fields low energy lattice oscillation (soft - phonon energy)High-dielectrics:High dielectric constantSmall bandgap
14Remote (SO) Phonon Scattering Coupling strength between the inversion layer electrons and the soft optical (SO) phonons (from the LO modes of insulator) Fröhlich interactionIonic polarizationElectronic polarizationStaticOptical (high frequency)SiO2 – small difference between andHigh- – large difference between andStrong SO phonon scattering degrades the inversion layer carrier mobility within the MOSFET with high- gate stacks.
15Monte Carlo simulations of Si MOSFET with HfO2 ID-VG characteristics of 67nm n-type Si MOSFET, with and without soft-optical phonon scattering from the HfO2 oxide.
16Monte Carlo simulations of strained Si MOSFET with HfO2ID-VG characteristics of 67nm n-type strained Si MOSFET with and without soft-optical phonon scattering from the HfO2 oxide.
17ObservationsWe observe that those simulations which include soft-optical phonon scattering exhibit a similar percentage reduction for both Si and strained Si n-MOSFETs at the same gate over drive VG-VT = 1.0V.The degradation in the drive current is ~40-50% at VD=0.1V and ~25% at VD=1.2V.SO phonon scattering decreases at high-drain voltages as the ‘Fröhlich’ interaction decreases with energy.
18Velocity profile along the channel Average channel velocities for the 67nm n-type bulk and strained Si MOSFETs, with and without soft-optical phonon scattering from the HfO2 gate stack.
19Monte Carlo simulations of Si MOSFET, with Al2O3ID-VG characteristics of 67nm n-type Si MOSFET, with and without soft-optical phonon scattering, from the Al2O3 oxide.
20Impact of high-k on Strained Si Source: Intel, IEDM 2003
21ConclusionsWe have investigated the impact on the performance degradation in sub 100nm n-MOSFETs due to soft-optical phonon scattering in the presence of high- dielectrics HfO2 and Al2O3.A device current degradation of around 25% at VG-VT=1.0V and VD=1.2V is observed for conventional and strained Si devices with a 2.2nm EOT HfO2. Correspondingly a current degradation of around 10% is observed for conventional and strained Si devices with a 2.2nm EOT Al2O3.Our results indicate that the performance degradation associated with high- gate stack MOSFETs can be compensated by the introduction of strained Si channels.The infancy of high- gate fabrication techniques means that overall performance degradation associated with high- gate dielectrics is expected to be worse than the predictions here.